The Harvard community has made this
article openly available. Please share how
this access benefits you. Your story matters
Citation Kaul, Ribhu K., Yong Baek Kim, Subir Sachdev, and T. Senthil. 2008. Algebraic charge liquids. Nature Physics 4(1): 28-31.
Published Version doi:10.1038/nphys790
Citable link http://nrs.harvard.edu/urn-3:HUL.InstRepos:7616534
arXiv:0706.2187v3 [cond-mat.str-el] 3 Dec 2007
Ribhu K. Kaul,1 Yong Baek Kim,2 Subir Sachdev,1 and T. Senthil3
Department of Physics, Harvard University, Cambridge MA 02138
Department of Physics, University of Toronto, Toronto, Ontario M5S 1A7, Canada
Department of Physics, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139
(Dated: June 2007)
High temperature superconductivity of the cuprates emerges upon changing the electron density of an insulator in which the electron spins are antiferro-magnetically ordered. A key characteristic of the superconductor  is that electrons can be extracted from them at zero energy only if their momenta take one of four specific values at the ‘nodal points’. A central enigma has been the evolution of the zero energy electrons in the metallic state between the anti-ferromagnet and the superconductor, and recent experiments yield apparently contradictory results. Resistance oscillations in a magnetic field [2, 3] indicate the zero energy electrons lie on elliptical ‘Fermi pockets’, while photoemission [4, 5] indicates they lie on arc-like regions. We describe new states of matter, called ‘algebraic charge liquids’, which arise naturally between the antiferro-magnet and the superconductor, and reconcile these observations. Our theory also explains the density of superconducting electrons, and makes a number of unique predictions for future experiments.
Soon after the discovery of high temperature superconductivity, Anderson  presented
influential ideas on its connection to a novel type of insulator, in which the electron falls
apart into emergent fractional particles which separately carry its spin and charge. These
ideas have been extensively developed , and can explain the nodal zero-energy electron
states in the superconductor. However, it is now known that the actual cuprate insulators
are not of this type, and instead have conventional antiferromagnetic order, with the electron
spins aligned in a checkerboard pattern on the square lattice. A separate set of ideas 
take the presence of antiferromagnetic order in the insulator seriously, but require a specific
effort to induce zero energy nodal electrons in the superconductor.
framework of ‘deconfined quantum criticality’  to describe the quantum fluctuations of
the electrons. We show how this framework naturally combines the virtues of the earlier
approaches: we begin with the antiferromagnetic insulator, but obtain electron
fractional-ization upon changing the electron density. A number of experimental observations in the
so-called ‘underdoped’ region between the antiferromagnet and the superconductor also fall
neatly into place.
A key characteristic of an ACL is the presence of an emergent fractional particle which
carries chargee, no spin, and has Fermi statistics. We shall refer to this fermion as a ‘holon’.
The holon comes in two species, carrying charges ±1 in its interaction with an emergent gauge field aµ, where µ is a spacetime index; this is a U(1) gauge field, similar to ordinary
electromagnetism. However, the analog of the electromagnetic fine structure constant is of
order unity for aµ, and so its quantum fluctuations have much stronger effects. We also
introduce operators f±† which create holons with charges ±1. ¿From the f± and aµ we can construct a variety of observables whose correlations decay with a power-law as function
of distance or time in an ACL. These include valence-bond-solid and charge-density wave
orders similar to those observed in recent scanning-tunnelling microscopy experiments .
While thef± carry the charge of the electron in the ACL, the spin of the electron resides
on another fractional particle, the ‘spinon’, with field operator zα where α=↑,↓is the spin index. The spinon is electrically neutral, and also carries aµ gauge charge. In an ACL, the
spinon is simply related to the antiferromagnetic order parameter; if ˆn is the unit vector
specifying the local orientation of the checkerboard spin ordering, then ˆn =z†~σz, where ~σ
are the Pauli matrices.
The nomenclature ‘ACL’ signals a formal connection to the previously studied insulating
‘algebraic spin liquids’ [9, 11, 12, 13, 14] which have power-law spin correlations, and of which
the deconfined critical point is a particular example. However, the observable properties of
the ACLs are completely different, with the ‘algebraic’ (or, equivalently ‘critical’) correlations
residing in the charge sector.
We begin our more detailed presentation of the ACLs by first considering the simpler state
in which long-range antiferromagnetic order is preserved, but a density x of electrons (per
Cu atom) have been removed from the insulator. This is the AF Metal of Fig. 1. This state
has been extensively discussed and well understood in the literature, and its properties have
electron creates a charge e, spin S = 1/2 fermionic ‘hole’ (to be distinguished from the
spinless ‘holon’) in the antiferromagnetic state. It is known that the momenta of the holes
reside in elliptical Fermi pockets centered at the pointsKi = (±π/2a,±π/2a) in the square lattice Brillouin zone (of lattice spacing a) - see Fig 2. This is a conventional metallic state,
not an ACL, with hole-like zero energy excitations (or equivalently, the hole ‘Fermi surface’)
along the dashed lines in Fig 2. In such a state, both the oscillations of the resistance as a
function of applied magnetic field (SdH for Shubnikov-de Haas)and emission of electrons by light (ARPES for angle-resolved photoemission) would indicate zero energy electron states
at the same momenta: along the dashed lines in Fig 2.
Now let us destroy the antiferromagnetic order by considering the vicinity of the
decon-fined critical point in the insulator . Arguments were presented in Ref.  that we obtain
a stable metallic state in which the electron fractionalizes into particles with precisely the
quantum numbers of the f± and the zα described above. This is the holon metal phase: a similar phase was discussed in early work by Lee , but its full structure was clarified
recently . Below we will discuss the properties of the holon metal, and of a number of
other ACLs that descend from it.
(i) Holon metal.
There is full spin rotation symmetry, and a positive energy (the spinon energy gap) is
required to create a zα spinon. The zero energy holons inherit the zero energy hole states
of the AF Metal, and so they reside along the dashed elliptical pockets in Fig 2, and these
will yield SdH oscillations characteristic of these pockets . However, the view from
ARPES experiments is very different—the distinction between SdH and ARPES views is a
characteristic property of all ACLs. The physical electron is a composite ofzαandf±, and so
the ARPES spectrum will have no zero energy states, and only a broad absorption above the
spinon energy gap. The frequencyF of the SdH oscillations is given by the Onsager-Lifshitz
F = Φ0A/(2π2), (1)
where Φ0 = hc/(2e) is the flux quantum, and A is the area in momentum space enclosed
Luttinger relation: there are 4 independent holon pockets, and the area of each pocket is
Aholon = (2π)2x/(4a2). (2)
(ii) Holon-hole metal
This is our candidate state for the normal state of the cuprates at low hole density (see
Fig 1). It is obtained from the holon metal when some of the holons and spinons bind to
form a charge e, S = 1/2 particle, which is, of course, the conventional hole, neutral under
the aµ charge. This binding is caused by the nearest-neighbor electron hopping, and the
computation of the dispersion of the bound state is described in the supplement. Now the
metal has both holons and hole charge carriers, and both have independent zero energy
states, i.e. Fermi surfaces. These Fermi surfaces are shown in Fig. 2, and both enclosed areas will contribute a SdH frequency via Eq. (1). The values of the areas depend upon
specific parameter values, but the Luttinger relation does yield the single constraint
Aholon+ 2Ahole= (2π)2x/(4a2); (3)
the factor of 2 prefactor of Ahole is due to S = 1/2 spin of the holes. This relation can offer
an explanation of the recent experiment  which observed SdH oscillations at a frequency
of 530T. We propose that these oscillations are due to the holon states. The holon density
may then be inferred to be 0.076 per Cu site while the total doping is x= 0.1. The missing
density resides in the hole pockets, which by Eq. (3) will also exhibit oscillations at the
frequency associated with the area [(2π)2/(4a2)]×0.012. The presence of SdH oscillations
at this lower frequency is a key prediction of our theory which we hope will be tested
experimentally. ARPES experiments detect only the hole Fermi surface, i.e. the ‘bananas’ in Fig. 2. With a finite momentum width due to impurity scattering, and the very small area
of each banana, the holon-hole metal also accounts for the arc-like regions observed in current
ARPES experiments [1, 4, 5]. Furthermore, because the nearest neighbor electron hopping
is suppressed by local antiferromagnetic correlations, we expect the binding to increase with
temperature, and this possibly accounts for the observed temperature dependence of the
Upon lowering the temperature in the holon metal, the holons pair to form a composite
boson which is neutral under theaµ charge, and the condensation of this boson leads to the
holon superconductor. Just as we determined the holon dispersion in the holon metal phase
by referring to previous work in the proximate AF metal, we can determine the nature of
the pair wavefunction by extrapolating from the state with co-existing antiferromagnetism
and superconductivity in Fig 1. The latter state was studied by Sushkov and collaborators
[18, 19], and they found that holes paired withd-wave symmetry. Hence the AF+dSC state
in Fig 1. We assume that the same pairing amplitude extends into the ACL obtained by
restoring spin rotation symmetry and inducing a spinon energy gap. The resulting holon
superconductor is not smoothly connected to the conventional BCS d-wave superconductor
because of the spin gap. The theory describing the low energy excitations of the holons in
the holon superconductor is developed in the supplement: it is found to be a mathematical
structure know as a conformal field theory (CFT). The present CFT has the U(1) gauge
field aµ coupled minimally to N = 4 species of Dirac fermions, ψi (i = 1. . . N), which are
descended from the f± holons after pairing. Such CFTs have been well-studied in other
contexts [11, 12, 13, 20]. For us, the important utility of the CFT is that it allows us to
compute the temperature (T) and x dependence of the density of superfluid electron, ρs
(measured in units of energy through its relation to the London penetration depth, λL by
ρs = ¯h2c2d/(16πe2λ2L), with d the spacing between the layers in the cuprates). For this, we
need the coupling of the CFT to the vector potential A~ of the electromagnetic field: this is
studied in the supplement and has the form~j·A~ where~j is a conserved ‘flavor’ current of the Dirac fermions ψi. The T dependence of ρs is then related to the T dependence of the
susceptibility associated with~j: such susceptiblities were computed in Ref. . In a similar
manner we found that as T →0 at small x
ρs(x, T) =c1x− RkBT (4)
where c1 is a non-universal constant and R is a universal number characteristic of CFT.
Remarkably, such a ρs is seen in experiments [22, 23, 24] on the cuprates over a range of
T and x. The phenomenological importance of such a ρs(x, T) was pointed out by Lee and
Wen , although Eq. (4) has not been obtained in any earlier theory . The holon
analyzed the CFT in a 1/N expansion and obtained
R= 0.4412 + 0.307(2)
N . (5)
We note that in the cuprates, there is a superconductor-insulator transition at a non-zero
x=xc, and in its immediate vicinity distinct quantum critical behavior ofρs is expected, as
has been observed recently. However, in characterizing different theories of the
under-doped regime, it is useful to consider the behavior asx→0 assuming the superconductivity survives untilx= 0. In this limit, our present theory is characterized bydρs/dT ∼constant, while theories of Refs. [27, 28] have dρs/dT ∼x2.
(iv) Holon-hole superconductor.
This is our candidate state of the superconductor at low hole density (see Fig 1). It is
obtained from a pairing instability of the holon-hole metal, just as the holon superconductor
was obtained from the holon metal. It is a modified version of the holon superconductor,
which has in addition low energy excitations from the paired holes. The latter will yield
the observed V-shaped spectrum in tunneling measurements. The holon-hole metal will also
have a residual metallic thermal conductivity at low T in agreement with experiment. For
ρs(x, T) we will obtain in addition to the terms in Eq. (4), a contribution from the nodal
holes to dρs/dT. This contribution can be computed using the considerations presented in
Refs. [26, 27]: it has only a weakx-dependence coming from the ratio of the velocities (which
can in principle be extracted from ARPES) in the two spatial directions. In particular, the
holes carry a current ∼ 1 and not ∼ x; the latter is the case in other theories [27, 28] of electron fractionalization which consequently have dρs/dT ∼x2.
Perhaps the most dramatic implication of these ideas is the possibility that the
supercon-ducting ground state of the underdoped cuprates is not smoothly connected to the
conven-tional superconductors described by the theory of Bardeen, Cooper, and Schrieffer(BCS).
With the reasonable additional assumption that such a BCS ground state is realized in
the overdoped cuprates, it follows that our proposal requires at least one quantum phase
We represent the electron operator on square lattice site r and spin α=↑,↓ as
crα ∼ fr†zrα r∈A (6)
rβ r∈B (7)
where A, B are the 2 sublattices, and εαβ is the unit antisymmetric tensor. The fr are
spinless charge-efermions carrying opposite aµ gauge charge±1 on the 2 sublattices. They will be denoted f± respectively. The effective action of the doped antiferromagnet on the
square lattice has the structure
S = Sz +Sf +St
g |∂τz| 2
g′ (z ∗
rzr′ + c.c.)
fs†(K) (∂τ +ǫK −µh)fs(K)
Z dτ κ0
c†rcr′ + c.c., (8)
where K is a momentum extending over the diamond Brillouin zone in Fig. 2. Sz is the lattice action for spinons. Sf describes holons hopping on the same sublattice, preserving the sublattice index s=±1; the holon dispersion ǫK has minima at theKi, andµh is the holon chemical potential. The first term in St describes an on-site electron chemical potential; the second to opposite sublattice electron hopping between nearest neighbors; the coupling
κ is expected to be significantly renormalized down by the local antiferromagnetic order
from the bare electron hopping element t. We have not included the aµ gauge field in the
above action which is easily inserted by the requirements of gauge invariance and minimal
For small g, g′, the z
α condense, and we obtain the familiar AF Metal state with hole
pockets (see Fig. 1). For larger g, g′ we reach the holon metal phase , in which the z
are gapped. The St term leads to two distinct (but not exclusive) instabilities of the holon
metal phase: towards pairing of the f± holons and the formation of bound states between
the holons and spinons. These lead, respectively, to the holon superconductor and the
will also significantly modify the spin correlation spectrum, likely inducing incommensurate
spin correlations , but this we will not address here.
Consider, first, the instability due to pairing between opposite gauge charges, hf+†f−†i 6= 0 so that the order parameter carries physical charge 2e, spin 0, and gauge charge 0. The aµ
gauge symmetry remains unbroken. The low energy theory of the holon superconductor has
gapless nodal Dirac holons ψi coupled to the gauge field aµ with the action
Sholon superconductor = Z
dτ d2R "
Here µ, ν, λ, ... are spacetime indices (τ, X, Y), and Dµ =∂µ−iaµ. This describes massless QED3 theory with N = 4 species of 2-component Dirac fermions which flows (within a 1/N
expansion) at low energies to a stable fixed point [11, 12] describing a CFT.
As the superconductivity arises through pairing of holons from a Fermi surface of area
∝ x, the superfluid density ρs(x,0) ∝ x. At T > 0 we need to include thermal excitation of unpaired holons, which are coupled to the vector potentialA~ of the physical
~ A· ∂ǫki
iksfiks ≡~j. ~A
In terms of the Dirac fermions these are readily seen to correspond to conserved “charges” of Eq. (9). The susceptibility associated with these charges is ∝ T , and so we obtain Eqn. 4.
Next we consider the κ-induced holon-spinon binding in the holon metal which leads to
the appearance of the holon-hole metal at low temperatures. St is a momentum dependent attractive contact interaction proportional to κ0 −κγK, with γK = (cos(Kx) + cos(Ky)) between a holon and spinon with center-of-mass momentum K We discuss the energy of
a bound holon-spinon composite using a non-relativistic Schrodinger equation assuming
initially that only a single holon is injected into the paramagnet and ignoring gauge
inter-actions. Consider a single holon valley (say valley 1). Taking a parabolic holon dispersion
with~k =K~ −K~1, and a spinon dispersion
Es(~k) = ∆s+ k
centered at (0,0) the energy of the holon-spinon composite will be
Eh(~k) = k
2M + ∆s−Ebind(~k) (12)
where M =mh+ ∆s. Define
with φ±(~r) the wavefunctions of a composite of a±-holon and a spinon separated by~r and
with center-of-mass momentum ~k. This satisfies the Schrodinger equation
φ =−Ebindφ (14)
whereρ=mh∆s/(mh+ ∆s) and ˜γ(k) =γ(K~1+~k) =−(sinkx+ sinky). (σxis a Pauli matrix acting on φ.) For the momenta of interest, this gives a~k-dependent hole binding energy
Ebind(1) ≈V0−V1γ˜(~k) (15)
with V0, V1>0. Thus the dispersion for h1 becomes
Eh1(~k) = k2
2M + ∆s−V0+V1γ˜(~k) (16)
The minimum ofEh1 is at a non-zero energy. Further as a function ofkX = (kx+ky)/2 it is
shifted along the positivekX direction by an amount 2MV1cos(kY) withkY = (−kx+ky)/2. Considering both holon and hole bands, it is clear that with increasing doping both bands
will be occupied to get a holon-hole metal. In the full Brillouin zone h1 is at momentum
−K~1 so that the hole Fermi surface lies entirely inside the diamond region and has the rough
banana shape shown in Fig. 2. The gauge interaction can now be included and leads to the
properties discussed in the main text.
Correspondence and request for materials to T. Senthil (firstname.lastname@example.org). We thank
Eric Hudson, Alessandra Lanzara, Patrick Lee, Mohit Randeria, Louis Taillefer, Ziqiang
Wang, Zheng-Yu Weng, and Xingjiang Zhou for many useful discussions. This research
DMR-0541988 (RKK), the NSERC (YBK), the CIFAR (YBK), and The Research
 A. Damascelli, Z. Hussain, and Z.-X. Shen,Angle-resolved photoemission studies of the cuprate superconductors,Rev. Mod. Phys.75, 473-541 (2003).
 N. Doiron-Leyraudet al.,Quantum oscillations and the Fermi surface in an underdoped high-Tc superconductor,Nature 447, 565-568 (2007).
 E. A. Yelland et al., Quantum Oscillations in the Underdoped Cuprate YBa2Cu4O8, arXiv:0707.0057.
 M. R. Norman et al., Destruction of the Fermi surface underdoped high-Tc superconductors,
Nature 392, 157-160 (1998).
 A. Kanigel et al., Evolution of the pseudogap from Fermi arcs to the nodal liquid, Nature Physics 2, 447-451 (2006).
 P. W. Anderson, The Resonating Valence Bond State in La2CuO4 and Superconductivity
,Science 235, 1196-1198 (1987).
 P. A. Lee, N. Nagaosa, and X.-G. Wen,Doping a Mott insulator: Physics of high-temperature superconductivity,Rev. Mod. Phys.78, 17-86 (2006).
 S. A. Kivelsonet al.,How to detect fluctuating stripes in the high-temperature superconductors,
Rev. Mod. Phys. 75, 1201-1241 (2003).
 T. Senthilet al.,Deconfined quantum critical points, Science 303, 1490-1494 (2004).
 Y. Kohsakaet al.,An Intrinsic Bond-Centered Electronic Glass with Unidirectional Domains in Underdoped Cuprates ,Science 315, 1380-1385 (2007).
 W. Rantner and X.-G. Wen,Electron spectral function and algebraic spin liquid for the normal state of underdoped high Tc superconductors, Phys. Rev. Lett.86, 3871-3874 (2001).
 M. Hermele et al.,Stability of U(1) spin liquids in two dimensions,Phys. Rev. B 70, 214437 (2004).
 M. Hermele, T. Senthil, and M. P. A. Fisher, Algebraic spin liquid as the mother of many competing orders, Phys. Rev. B 72104404 (2005).
 R. K. Kaul et al.,Hole dynamics in an antiferromagnet across a deconfined quantum critical point,Phys. Rev. B 75, 235122 (2007).
 P. A. Lee, Gauge field, Aharonov-Bohm flux, and high-Tc superconductivity,Phys. Rev. Lett.
63, 680-683 (1989).
 Y. B. Kim, P. A. Lee, and X.-G. Wen, Quantum Boltzmann equation of composite fermions interacting with a gauge field,Phys. Rev. B 52, 17275-17292 (1995).
 V. V. Flambaum, M. Yu. Kuchiev, and O. P. Sushkov,Hole-Hole superconducting pairing in the t-J model induced by long-range spin-wave exchange,Physica C 227, 267-278 (1994).  V. I. Belinicheret al.,Hole-Hole superconducting pairing in the t-J model induced by spin-wave
exchange,Phys. Rev. B 51, 6076-6084 (1995).
 O. Vafek, Z. Tesanovic, and M. Franz, Relativity restored: Dirac anisotropy in QED3,Phys. Rev. Lett. 89, 157003 (2002).
 A. V. Chubukov, S. Sachdev, and J. Ye, Theory of two-dimensional quantum Heisenberg antiferromagnets with a nearly critical ground state,Phys. Rev. B 49, 11919-11961 (1994).  D. A. Bonnet al.,Surface impedance studies ofYBCO,Czech. J. Phys.46, 3195-3202 (1996).  B R. Boyce, J. Skinta, and T. Lemberger,Effect of the pseudogap on the temperature
depen-dence of the magnetic penetration depth in YBCO films,Physica C 341-348, 561 (2000).  M. Le Taconet al.,Two Energy Scales and two Quasiparticle Dynamics in the Superconducting
State of Underdoped Cuprates,Nature Physics 2, 537-543 (2006).
 I. Hetel, T. R. Lemberger, and M. Randeria, Quantum critical behaviour in the super-fluid density of strongly underdoped ultrathin copper oxide films, Nature Physics online, doi:10.1038/nphys707.
 P. A. Lee and X.-G. Wen, Unusual superconducting state of underdoped cuprates,Phys. Rev. Lett. 78, 4111-4114 (1997).
 C. P. Nave, D. A. Ivanov, and P. A. Lee, Variational Monte Carlo study of the current carried by a quasiparticle,Phys. Rev. B 73, 104502 (2006).
 P. W. Andersonet al., The Physics Behind High-Temperature Superconducting Cuprates: The “Plain Vanilla” Version Of RVB, J Phys. Condens. Matter16, R755-R769 (2004).
 B. I. Shraiman and E. D. Siggia,Mobile Vacancies in a Quantum Heisenberg Antiferromagnet
algebraic charge liquid
FIG. 1: Schematic phase diagram at smallx. HereT is the temperature, andx is the density
of electrons (per Cu atom) which have been removed from the insulator. The phases labelled “AF”
have long-range antiferromagnetic order. The AF+dSC state also has d-wave superconductivity
and was described in Ref. [18, 19]. For the cuprates, we propose that the ACL phase above
is a holon-hole metal, while the superconducting ACL is the holon-hole superconductor. The
FIG. 2: Square lattice Brillouin zone containing the ‘diamond’ Brillouin zone (dashed
line). In the AF Metal, only the dashed ellipses are present, and they represent Fermi surfaces
of S = 1/2, charge e holes which are visible in both ARPES and SdH. In the holon metal, these
dashed ellipses become spinless charge e holon Fermi surfaces, and are visible only in SdH. The
full line ‘bananas’ are the hole Fermi surfaces present only in the holon-hole metal, and detectable